Fundamentals of Corrosion. ACADs (08-006) Covered Keywords Description Supporting Material. Fundamentals of Corrosion. Prepared by Ivelisse Ortiz-Hernandez, PhD. Source: File h1015v1 from the DOE, Module 2. Objectives.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Fundamentals of Corrosion
ACADs (08-006) Covered
Augusta Technical College2011
Fundamentals of Corrosion
Ivelisse Ortiz-Hernandez, PhD.
Source: File h1015v1 from the DOE, Module 2
e. General corrosion
There are two types of electrochemical cells: galvanic (ones that spontaneously produce electrical energy) and electrolytic (ones that consume electrical energy).
A potential difference between two electrodes represents a tendency for the reaction to occur.
Example of a REDOX reaction
Wastage Corrosion Tests
As Zn+2 increases and Cu+2 decreases, the electrical potential decreases.
This decrease in cell potential, which results from changes in concentrations, is one form of polarization called concentration polarization.
Again, as the cell operates, the cell
The decrease is partially due to the increase in Zn+2 concentration and the decrease in H3O+ concentration.
The second type of polarization is associated with the reduction half-reaction.
Hydrogen ion remains in the surface of the Pt electrode until it either recombines with a second hydrogen atom to form molecular hydrogen, H2 or are removed by reacting with oxygen to form water.
The sites are blocked until the hydrogen is removed.
The protection provided by the film depends on the tenacity of the film.
A loosely attached film will continue to corrode. If defects develop in the film, corrosion will take place.
Corrosion layer is compromised at low and high pH at higher temperatures.
A pH between 7 and 10 gives a lower rate of corrosion.
The pH is always maintained alkaline to minimize corrosion rate.
Having hydrogen in the water helps minimize the amount of corrosion by eliminating the amount of oxygen in the system.
Dissolved oxygen reacts with the protective hydrogen gas layer at the cathode to form water.
Alloys used in a Nuclear System
Localized corrosion takes place a lot faster than general corrosion.
In extreme cases, failure with localized corrosion will take just days.
Only specific metals under specific conditions are susceptible to localized corrosion.
When a metal is subjected to a load (force), it is distorted or deformed, no matter how strong the metal or light the load.
Elastic strain – regains its shape
Plastic strain – if after the load is applied the shape is not regained.
The phenomenon of elastic strain and plastic deformation in a material are called elasticity and plasticity, respectively.
Atoms in a material are arranged in a specific geometry which depends in the intermolecular interactions.
To distort the pattern of a crystal, work most be done in the material.
Work = Force times the distance that the force moves
Stress is the internal resistance, or counterforce, of a material to the distorting effects of an external force or load.
Residual stresses are due to the manufacturing processes that leave stresses in a material. Welding leaves residual stresses in the metals welded.
Structural stresses are stresses produced in structural members because of the weights they support.
Pressure stresses are stresses induced in vessels containing pressurized materials.
Flow stresses occur when a mass of flowing fluid induces a dynamic pressure on a conduit wall. The force of the fluid striking the wall acts as the load.
Thermal stresses exist whenever temperature gradients are present in a material. Different temperatures produce different expansions and subject materials to internal stress.
Fatigue stresses are due to cyclic application of a stress. The stresses could be due to vibration or thermal cycling.
Tensile stress is that type of stress in which the two sections of material on either side of a stress plane tend to pull apart or elongate.
Compressive stress is the reverse of tensile stress.
Shear stress exists when two parts of a material tend to slide across each other in any typical plane of shear upon application of force parallel to that plane.
Compressibility is the ability of a material to react to compressive stress or pressure.
Stress Cracking Corrosion
Stress Cracking Corrosion
Occurs in all alloys
Stress corrosion cracking (SCC) is a type of intergranular attack corrosion that occurs at the grain boundaries under tensile stress.
Most pure metals are immune to this type of attack.
According to the most widely accepted theory, stress corrosion cracking is caused by a process called chemisorption. Unlike relatively weak physical absorption, such as hydrogen gas on platinum metal, chemisorption may be thought of as the formation of a compound between the metal atoms on the surface as a monomolecular layer of the chemisorbed substance, such as Cl-, OH-, Br-, and some other ions.
Conditions for this corrosion to exist
Susceptible metal alloy and a corroding substance
Oxygen in water
Temperature greater than 140 ºF
A large tensile stress is required for it to occur.
Stress Cracking Corrosion, cont.
The stress can come from service loads, residual stress from manufacturing processes, mismatch of components during construction, or a wedging action due to accumulation of corrosion products.
Once a stress is present, the other factors must also be present for corrosion to occur.
A defect initially present then grows as the metal atoms separate under stress, more chemisorption occurs, and the process continues.
Stainless steels containing 18 percent chromium and 8 percent nickel are susceptible to cracking in environments containing chloride ions and in concentrated caustic environments (that is, in environments where the hydroxyl ion concentration is high).
If the environment is severe enough, cracking can occur in a very short period of time.
Stress Cracking Corrosion, cont.
Careful fabrication of plant components
Maintain chloride, fluoride and oxygen content below the specified limits.
If oxygen is kept at very low limits, then higher chloride and fluoride limits can be tolerated.
The reverse is also true.
Occurs in zircalloy and ferrous metal (iron containing metals).
Concentrated Caustic conditions (pH close to 14)
Difference between tensile stress corrosion and caustic corrosion is the chemicals involved to start the reaction.
Under very caustic conditions, corrosion rate increases (pH = 14)
pH should be maintained between 7 and 10
To minimize general corrosion of most metal a pH of 7 or greater.
pH = 11.3 – zircaloy corrosion layer is dissolved (pH must be maintained below 11.3 to ensure that the zircaloy layer is protected)
Exposure of the zircaloy structure increases the chances of zirc-hydriding.
The concentrated basic conditions are caused by boiling (basic solution concentrates in crevices). The caustic material plates out of solution. When it is remoistened it creates a region with a highly caustic environment.
Improved resistance to caustic stress corrosion cracking can be given to Inconel by heat treating it at 620ºC to 705ºC, depending upon prior solution treating temperature.
Strict pH control is the only solution.
Materials cannot be changed and boiling cannot be avoided.
Corrosion for Inconel
Following the grain boundaries
Corrosion for 316 stainless steel
Two dissimilar metals in contact of electrically conductive water.
One of the metals can develop accelerated corrosion.
The metals must have a different electric potentialfor the reaction to occur.
The difference in potential creates a small current (flow of electrons).
The metal with the lower oxidation potential readily oxidizes in water.
Two dissimilar metals in contact
Oxygen dissolved in water
Both Cu and Zn are oxidized in the presence of oxygen in water.
The electric potential of copper is 1.90 and for zinc is 1.65.
Electrons flow from least potential to higher potential.
Copper does not corrode and zinc corrodes at an accelerated pace.
To minimize it
Use corrosion resistant materials
Use materials with similar electronegativity. For example: Cupper and Nickel: 1.90 and 1.91.
Use sacrificial anode (to corrode this material intentionally)
Use a transition piece between the metals (the transition piece must have similar properties than the two metals.
Prevented by minimizing the oxygen content in water.
Is a type of galvanic corrosion.
Involves two pieces of the same metal.
Conditions for it to occur
Two closely fitted parts
Soluble salts or oxygen in water.
Occurs if a difference in oxygen concentration or salt concentration exist between the crevice and the surface.
The increase concentration of salt in the crevice increases the corrosion in this area.
In stage three of the crevice development a few more accelerating factors fully develop:
The metal ions produced by the anodic corrosion reaction readily hydrolyze giving off protons (acid) and forming corrosion products. The pH in a crevice can reach very acidic values, sometimes equivalent to pure acids.
The acidification of the local environment can produce a serious increase in the corrosion rate of most metals. See, for example, how the corrosion of steel is affected as a function of water pH.
The corrosion products seal even further the crevice environment.
The accumulation of positive charge in the crevice becomes a strong attractor to negative ions in the environment, such as chlorides and sulfates, that can be corrosive in their own right.
Keep water very pure.
Soluble salt and oxygen must be minimized.
Larger crevices (to minimize high concentration areas)
Continuous movement of the parts will minimize it.
Air (or oxygen) is bubbled around one electrode, and nitrogen is bubbled around the other. A current flows through the wire connecting the two electrodes.
The difference in potential is a result of the difference in oxygen concentration at the two electrode surfaces.
At the electrode exposed to nitrogen, electrons are given up by the iron as it is oxidized.
As a result, oxidation occurs at the electrode exposed to nitrogen and reduction occurs at the aerated electrode. Corrosion takes place in the oxygen free area and reduction takes place in the cathode.
Caused by inconsistencies in material composition of the metal and the presence of oxygen and fluoride or chloride.
When the material has differences in potential in nearby portions corrosion can occur.
Oxygen attacks the area most prone to corrosion. The presence of chlorides accelerate the corrosion rate.
Corrosion forms a pit that can eventually cause a rupture.
Minimize by using homogeneous metals and minimizing the presence of oxygen and chloride in solution.
Low chloride concentration
Low fluoride concentration
Low oxygen concentration
Neutral to moderate basic pH
Avoid heavy metals like mercury